Issued by RPP-WTP PDC · PDF file...
Embed Size (px)
Transcript of Issued by RPP-WTP PDC · PDF file...
Issued by RPP-WTP PDC
24590-LAW-N1D-LVP-00002 Rev. 4
LVP-TK-00001: Sheet: 2 of 14
Complete re-write; no rev bars shown New format
Incorporate revised PCDS Update references DLAdler APRangus RBDavis TErwin
2 5/25/05 Update wear allowance based on 24590-WTP-RPT-M-04-0008 DLAdler JRDivine NA APRangus
Change item number from VSL to TK Correct description
Update design temp/pressure Incorporate new PCDS
Information regarding inadvertent nitric acid addition
Re-format references Add DWP note DLAdler JRDivine
APRangus 0 3/6/02 Initial Issue JRDivine DLAdler NA SKirk
REV DATE REASON FOR REVISION ORIGINATE CHECK REVIEW APPROVE Please note that source, special nuclear and byproduct materials, as defined in the Atomic Energy Act of 1954 (AEA), are regulated at the U.S. Department of Energy (DOE) facilities exclusively by DOE acting pursuant to its AEA authority. DOE asserts that pursuant to the AEA, it has sole and exclusive responsibility and authority to regulate source, special nuclear, and byproduct materials at DOE- owned nuclear facilities. Information contained herein on radionuclides is provided for process description purposes only. This bound document contains a total of 14 sheets.
24590-LAW-N1D-LVP-00002 Rev. 4
LVP-TK-00001: Sheet: 3 of 14
Corrosion/Erosion Detailed Discussion The caustic collection tank is designed to hold caustic scrub solution, control pH by addition of 5 molar NaOH, and control precipitation by addition of process service water (PSW). Where the text of the Process Corrosion Data report attached describes the transfer of liquid effluents to RLD-VSL-00017A/B for the baseline configuration, it should also include the transfer of liquid effluents to DEP-VSL-00004A/B under the DFLAW configuration. 1 General/Uniform Corrosion Analysis a Background General corrosion or uniform corrosion is corrosion that is distributed more-or-less uniformly over the surface of a material without appreciable localization. This leads to relatively uniform thinning on sheet and plate materials and general thinning on one side or the other (or both) for pipe and tubing. It is recognized by a roughening of the surface and by the presence of corrosion products. The mechanism of the attack is an electrochemical process that takes place at the surface of the material. Differences in composition or orientation between small areas on the metal surface create anodes and cathodes that facilitate the corrosion process. b Component-Specific Discussion Based on the applicable PCDS, the tank contains alkaline scrub solution at operating temperature of 122 °F. Due to normal design evolution, the source calculation referenced by the PCDS has been revised lowering the normal temperature of the tank contents to 118 °F and showing the maximum operating temperature to be 123 °F. The difference in operating temperatures between the two documents has been considered and found insignificant. This evaluation will continue based on the temperature shown in the PCDS, 122 °F. Either type 304L or type 316L is expected to be sufficiently resistant to water. The uniform corrosion rate is low under these conditions. A 0.04 inch total corrosion allowance is recommended; 0.024 inch allowance for uniform corrosion (24590-WTP-M0C-50-00004, Wear Allowance for WTP Waste Slurry Systems). 2 Pitting Corrosion Analysis Pitting is localized corrosion of a metal surface that is confined to a point or small area and takes the form of cavities. Chloride is known to cause pitting in acid and neutral solutions. Normally the tank is to operate at 122 °F at a pH of 9.5. The tank is operated such that conditions do not promote localized corrosion. The tank contents are not stagnant. The expected chemistry and temperature in this tank fall within the limits for localized corrosion established for 300 series stainless steel in Table 18-1 of 24590-WTP-DB-ENG-01-001. 3 Crevice Corrosion Analysis Crevice corrosion is a form of localized corrosion of a metal or alloy surface at, or immediately adjacent to, an area that is shielded from full exposure to the environment because of close proximity of the metal or alloy to the surface of another material or an adjacent surface of the same metal or alloy. Crevice corrosion is similar to pitting in mechanism. It can, however, be initiated at lower temperatures than is pitting. Crevices in this tank are limited by the design and fabrication practice. The expected chemistry and temperature in this tank fall within the limits established for Type 316L in Table 18-1 of 24590-WTP-DB-ENG-01-001. 4 Stress Corrosion Cracking Analysis Stress corrosion cracking (SCC) is the cracking of a material produced by the combined action of corrosion and sustained tensile stress (residual or applied). The exact amount of chloride required to cause stress corrosion cracking is unknown. In part this is because the amount varies with temperature, metal sensitization, and the environment. But it is also unknown because chloride tends to concentrate under heat transfer conditions, by evaporation, and electrochemically during a corrosion process. Hence, even as little as 10 ppm can lead to cracking under some conditions. Generally, as seen in Sedriks (1996) and Davis (1987), stress corrosion cracking does not usually occur below about 140°F for sensitized alloys. The expected chemistry and temperature in this tank fall within the limits established for Type 316L in Table 18-1 of 24590-WTP-DB- ENG-01-001. 5 End Grain Corrosion Analysis End grain corrosion is preferential aqueous corrosion that occurs along the worked direction of wrought stainless steels exposed to highly oxidizing acid conditions. End grain corrosion typically is not a major concern, it propagates along the rolling direction of the plate, not through the cross-sectional thickness. In addition, end grain corrosion is exclusive to metallic product forms with exposed end grains from shearing or mechanical cutting. Such conditions are not present in this system.
24590-LAW-N1D-LVP-00002 Rev. 4
LVP-TK-00001: Sheet: 4 of 14
6 Weld Corrosion Analysis The welds used in the fabrication will follow the WTP specifications and standards for quality workmanship. The materials selected for this fabrication are compatible with the weld filler metals and ASME/AWS practice. Using the welding practices specified for the project there should not be gross micro-segregation, precipitation of secondary phases, formation of unmixed zones, or volatilization of the alloying elements that could lead to localized corrosion of the weld. Assuming that correct weld procedures are followed, no preferential corrosion of weld beads or heat-affected zones occurs in nitric acid or alkaline-based stream. 7 Microbiologically Influenced Corrosion Analysis Microbiologically influenced corrosion (MIC) refers to corrosion affected by the presence or activity, or both, of microorganisms. The proposed operating conditions are suitable for microbial growth. However, treated process water is used and water quality is controlled to prevent MIC. 8 Fatigue/Corrosion Fatigue Analysis Corrosion-fatigue is the result of the combined action of cyclic stresses and a corrosive environment. The fatigue process is thought to cause rupture of the protective passive film, upon which stainless steel can actively corrode in the localized area of the film rupture. The corrosive environment may also act to reduce the stress necessary for film rupture. The result is that a metal exposed to a corrosive environment and cyclic mechanical load may initiate cracking at conditions at stress levels less than the endurance limit for the material. The conclusion that corrosion fatigue will not be a problem is based on the low mechanical and thermal cycling. 9 Vapor Phase Corrosion Analysis Conditions in the vapor phase and at the vapor/liquid interface can be significantly different than those present in the liquid phase. The vapor space corrosion rates are less than the immersed surfaces and the transport away from the surface will be less because of the no-flow conditions. As compared to the corrosion in the immersion section, the corrosion rates in the vapor space are much lower. Vapor phase corrosion is not a concern. 10 Erosion Analysis Erosion is the progressive loss of material from a solid surface resulting from mechanical interaction between that surface and a fluid, a multi-component fluid, or solid particles carried with the fluid. Velocities within the tank are expected to be below 12 ft/s and solids content negligible. Erosion allowance of 0.004 inch for components with low solids content (< 2 wt%) at low velocities is based on 24590- WTP-M0C-50-00004. 11 Galling of Moving Surfaces Analysis Where two metals are moving in contact with each other without lubrication, there is a risk of damage to their surfaces. No moving unlubricated surfaces are present within the tank; therefore, galling is not a concern. 12 Fretting/Wear Analysis Fretting corrosion refers to corrosion damage caused by a slight oscillatory slip between two surfaces. Similar to galling but at a much smaller movement, the corrosion products and metal debris break off and act as an abrasive between the surfaces, producing a classic three-body wear problem. This damage is induced under load and repeated relative surface mot